- Nano Express
- Open Access
One-Pot Green Synthesis and Bioapplication ofl-Arginine-Capped Superparamagnetic Fe3O4 Nanoparticles
© to the authors 2009
- Received: 14 September 2009
- Accepted: 28 October 2009
- Published: 13 November 2009
Water-solublel-arginine-capped Fe3O4 nanoparticles were synthesized using a one-pot and green method. Nontoxic, renewable and inexpensive reagents including FeCl3,l-arginine, glycerol and water were chosen as raw materials. Fe3O4 nanoparticles show different dispersive states in acidic and alkaline solutions for the two distinct forms of surface bindingl-arginine. Powder X-ray diffraction and X-ray photoelectron spectroscopy were used to identify the structure of Fe3O4 nanocrystals. The products behave like superparamagnetism at room temperature with saturation magnetization of 49.9 emu g−1 and negligible remanence or coercivity. In the presence of 1-ethyl-3-(dimethylaminopropyl) carbodiimide hydrochloride, the anti-chloramphenicol monoclonal antibodies were connected to thel-arginine-capped magnetite nanoparticles. The as-prepared conjugates could be used in immunomagnetic assay.
(See supplementary material 1)
- Amino acid
In the last decade, inherently safer nanomaterials and nanostructured devices were widely fabricated with the “green chemistry” principles [1–13]. It is important to design synthetic methodologies that possess the minimization or even total elimination toxicity to the environment and human health in green chemistry [1, 14]. The nontoxic, renewable raw materials and environmentally benign solvents are generally considered in a green synthetic strategy . As society and environment can benefit from the products, green chemistry can convey a responsible attitude to public toward the development of nanoscience and nanotechnology .
Magnetite (Fe3O4) nanoparticles have attracted intensive interests for a wide range of fields, including magnetic fluids, immobilization of proteins, peptides and enzymes, immunoassays, drug or gene delivery magnetic resonance imaging, data storage, environmental remediation [15–25]. The Fe3O4 nanoparticles perform best in most of biomedicinal applications when the size of the nanoparticles is around 10–20 nm. In this range, an individual nanoparticle becomes a single magnetic domain and shows superparamagnetic behavior above blocking temperature [26, 27]. Large numbers of methods have been developed for the synthesis of high-quality Fe3O4 nanoparticles of various surface modifier based on the thermal decomposition of iron organometallic compounds in a high-boiling point organic solvent [28–37]. When those magnetite nanoparticles are applied in biomedical fields, surface post-treatments are usually needed.
In the present work, we described a facile and green approach toward synthesis and stabilization of Fe3O4 nanoparticles. Water and glycerol were used as environmentally benign solvents in the synthesis. Inartificial amino acidl-arginine was chosen as the nontoxic, renewable stabilizing agent.
Chloramphenicol (CAP) and 1-ethyl-3-(dimethylaminopropyl) carbodiimide hydrochloride (EDC) were purchased from Sigma–Aldrich. o-Phenylenediamine (OPD) was purchased from Xinjingke Biotechnology. Hydrogen peroxide (30%) was supplied by Guangmang Chemical Co. The anti-CAP monoclonal antibody and HRP-CAP conjugates were produced by our lab. Other analytical grade chemicals were purchased from Shanghai Chemical Reagents Company. All of the chemicals were used as received without further purification.
Phosphate-buffered saline (PBS): 138 mM NaCl, 1.5 mM KH2PO4, 8 mM Na2HPO4·H2O and 2.7 mM KCl, pH = 7.4.
Washing buffer (PBST): PBS containing 0.05 (v/v) Tween 20.
Citrate buffer: 19 mM citric acid, 33.5 mM Na2HPO4·H2O, pH = 5.0
Substrate solution: 5 mg OPD, 12.5 mL citrate buffer, 2.5 μL H2O2(30%).
Stopping solution: 2 N HCl.
Synthesis ofl-Arginine-Capped Fe3O4Nanoparticles
l-Arginine (3.0 g) and FeCl3(0.5 g) were added to a component solvent containing glycerol (10 mL) and water (10 mL). A transparent solution formed through sonication of this mixture. This solution was transferred into a Teflon-lined stainless steel autoclave with a capacity of 50 mL and maintained at 200°C for 6 h. Then, the autoclave was cooled to room temperature naturally. The product was washed with distilled water to remove residue of solvent and unboundl-arginine, finally dried by vacuum freeze-desiccation technology before characterization. During each step, the product was separated from the suspension by magnetic force.
Preparation of Magnetic Nanoparticles Conjugates
A solution was formed by mixing 250 μL Fe3O4 nanoparticles suspension and 1 mL phosphate-buffered saline (PBS). Then, 10 μL of anti-CAP monoclonal antibody and 1 mg of 1-ethyl-3-(dimethylaminopropyl) carbodiimide hydrochloride (EDC) were added. Afterward, the mixture was incubated overnight with light shaking at room temperature. Excess EDC and the supernatant were removed by magnetic separation, and the precipitate was washed three times with PBS. Antibody-labeled magnetic nanoparticles were redispersed in PBS (1 mL) and stored at 4°C for use.
The above store suspension (100 μL) was added to a tube and rinsed three times with washing buffer (PBST) in a magnetic field. Then, 100 μL conjugates of chloramphenicol and horseradish peroxidase (CAP-HRP) were injected. The incubation was performed for 2 h at room temperature with constant shaking. The sample was washed three times with PBST as earlier. Substrate solution (100 μL) was added, and the reaction was kept for 15 min. Finally, stopping solution (2 N HCl) was used to stop the reaction, and the absorbance was determined at 492 nm. A comparative experiment was performed just replaced magnetic nanoparticles conjugates with unlabeled magnetic nanoparticles.
XRD patterns were recorded on the X-ray diffractometer (Bruker D8) with a graphite monochromator and Cu Kα radiation (λ = 1.5418 Å) in the range of 10–80° at room temperature. The morphology of the products was determined with transmission electron microscopy (JEM-100CXII) with an accelerating voltage of 80 kV. The nanocrystals dispersed in water were cast onto a carbon-coated copper grid. Magnetization measurements of the nanocomposites were performed with a Micromag 2900 at room temperature under ambient atmosphere. X-ray photoelectron spectra (XPS) were measured with X-Ray photoelectron spectroscopy XPS (ESCALAB 250). Enzyme immunoassay (ELISA) was performed with an automatic microplate reader KHB ST-360 from Shanghai Zhihua Medical Instrument Ltd.
We have synthesizedl-arginine-capped superparamagnetic Fe3O4 nanoparticles via a simple and green method in water and glycerol component solvent. The synthesized Fe3O4 nanoparticles have an average diameter of 13 nm and the saturation magnetization reaches to 49.9 emu g−1 with negligible remanence or coercivity. With superparamagnetic properties and the active groups on the surface of the nanoparticles, their application for magnetic separation and concentration in immunoassays were further demonstrated. These products are expected to have more extensive applications in biomedical fields.
Financial support from the Program for New Century Excellent Talents in University (NCET-06-0586), the Key Project of Chinese Ministry of Education (No. 109098), and the National Basic Research Program of China (973 Program 2005CB623601, 2007CB936602) is gratefully acknowledged. Prof. Xi acknowledges the financial support from the National Natural Science Foundation of China (No. 20675048), the National High-Tech Research and Developmental Program of China (863 Program, No. 07AA10Z435 and 2007AA06A407).
- Anastas PT, Warner JC: Green Chemistry: Theory and Practice. Oxford university Press Inc, New York; 1998.Google Scholar
- Matlack AS: Introduction to Green Chemistry. Marcel Decker, New York; 2001.Google Scholar
- Raveendran P, Fu J, Wallen SL: J. Am. Chem. Soc.. 2003, 125: 13940. COI number [1:CAS:528:DC%2BD3sXot12ms7k%3D] 10.1021/ja029267jView ArticleGoogle Scholar
- Raveendran P, Fu J, Wallen SL: Green Chem.. 2006, 8: 34. COI number [1:CAS:528:DC%2BD28XhsF2ntA%3D%3D] 10.1039/b512540eView ArticleGoogle Scholar
- Hu B, Wang SB, Wang K, Zhang M, Yu SH: J. Phys. Chem. C.. 2008, 112: 11169. COI number [1:CAS:528:DC%2BD1cXotVCltbo%3D] 10.1021/jp801267jView ArticleGoogle Scholar
- Shankar SS, Rai A, Ankamwar B, Singh A, Ahmad A, Sastry M: Nat. Mater.. 2004, 3: 482. COI number [1:CAS:528:DC%2BD2cXlt1Ors74%3D]; Bibcode number [2004NatMa...3..482S] 10.1038/nmat1152View ArticleGoogle Scholar
- Xie JP, Lee JY, Wang DIC, Ting YP: Small. 2007, 3: 672. COI number [1:CAS:528:DC%2BD2sXktFGntLk%3D] 10.1002/smll.200600612View ArticleGoogle Scholar
- Wang Y, Maksimuk S, Shen R, Yang H: Green Chem.. 2007, 9: 1051. 10.1039/b618933dView ArticleGoogle Scholar
- Mukherjee P, Ahmad A, Mandal D, Senapati S, Sainkar SR, Khan MI, Parishcha R, Ajaykumar PV, Alam M, Kumar R, Sastry M: Nano Lett.. 2001, 1: 515. COI number [1:CAS:528:DC%2BD3MXmt1OksL8%3D]; Bibcode number [2001NanoL...1..515M] 10.1021/nl0155274View ArticleGoogle Scholar
- Saito Y, Wang JJ, Smith DA, Batchelder DN: Langmuir. 2002, 18: 2959. COI number [1:CAS:528:DC%2BD38XhvFymtLw%3D] 10.1021/la011554yView ArticleGoogle Scholar
- Mukherjee P, Ahmad A, Mandal D, Senapati S, Sainkar SR, Khan MI, Parishcha R, Ajaykumar PV, Alam M, Kumar R, Sastry M: Angew. Chem. Int. Ed.. 2001, 40: 3585. COI number [1:CAS:528:DC%2BD3MXns1Wgsrw%3D] 10.1002/1521-3773(20011001)40:19<3585::AID-ANIE3585>3.0.CO;2-KView ArticleGoogle Scholar
- Yang JH, Lu LH, Wang HS, Shi WD, Zhang HJ: Cryst. Growth Des.. 2006, 6: 2155. COI number [1:CAS:528:DC%2BD28XnsFemur8%3D] 10.1021/cg060143iView ArticleGoogle Scholar
- Nadagouda MN, Varma RS: Green Chem.. 2006, 8: 516. COI number [1:CAS:528:DC%2BD28Xltlars70%3D] 10.1039/b601271jView ArticleGoogle Scholar
- Jennifer AD, Bettye LSM, James EH: Chem. Rev.. 2007, 107: 2228. 10.1021/cr050943kView ArticleGoogle Scholar
- Neuberger T, Schöpf B, Hofmann H, Hofmann M, von Rechenberg BJ: J. Magn. Magn. Mater.. 2005, 293: 483. COI number [1:CAS:528:DC%2BD2MXktVagsbo%3D]; Bibcode number [2005JMMM..293..483N] 10.1016/j.jmmm.2005.01.064View ArticleGoogle Scholar
- Liu JF, Zhao ZS, Jiang GB: Environ. Sci. Technol.. 2008, 42: 6949. COI number [1:CAS:528:DC%2BD1cXpvVSisLw%3D] 10.1021/es800924cView ArticleGoogle Scholar
- Wang LY, Bao J, Wang L, Zhang F, Li YD: Chem. Eur. J.. 2006, 12: 6341. COI number [1:CAS:528:DC%2BD28XptV2ntL4%3D] 10.1002/chem.200501334View ArticleGoogle Scholar
- Xu C, Xu K, Gu H, Zhong X, Guo Z, Zheng R, Zhang X, Xu B: J. Am. Chem. Soc.. 2004, 126: 3392. COI number [1:CAS:528:DC%2BD2cXhsFyitrw%3D] 10.1021/ja031776dView ArticleGoogle Scholar
- Jia X, Chen DR, Jiao XL, Zhai SM: Chem. Commun.. 2009, 8: 968. 10.1039/b813524jView ArticleGoogle Scholar
- Shi QX, Lu RW, Jin K, Zhang ZX, Zhao DF: Green Chem.. 2006, 8: 868. COI number [1:CAS:528:DC%2BD28XhtVCiu7rE] 10.1039/b606705kView ArticleGoogle Scholar
- Dyal A, Loos K, Noto M, Chang SW, Spagnoli C, Shafi KVPM, Ulman A, Cowman M, Gross RA: J. Am. Chem. Soc.. 2003, 125: 1684. COI number [1:CAS:528:DC%2BD3sXmslaktQ%3D%3D] 10.1021/ja021223nView ArticleGoogle Scholar
- Mirzabekov T, Kontos H, Farzan M, Marasco W, Sodroski J: Nat. Biotechnol.. 2000, 18: 649. COI number [1:CAS:528:DC%2BD3cXktlSktbo%3D] 10.1038/76501View ArticleGoogle Scholar
- Won J, Kim M, Yi YW, Kim YH, Jung N, Kim TK: Science. 2005, 309: 121. COI number [1:CAS:528:DC%2BD2MXlsF2htro%3D]; Bibcode number [2005Sci...309..121W] 10.1126/science.1112869View ArticleGoogle Scholar
- Kotani M, Koike T, Yamaguchi K, Mizuno N: Green Chem.. 2006, 8: 735. COI number [1:CAS:528:DC%2BD28XnsFyitLs%3D] 10.1039/b603204dView ArticleGoogle Scholar
- Ge JP, Hu YX, Biasini M, Dong CL, Guo JH, Beyermann WP, Yin YD: Chem. Eur. J.. 2007, 13: 7153. COI number [1:CAS:528:DC%2BD2sXhtVeltbnN] 10.1002/chem.200700375View ArticleGoogle Scholar
- Lu AH, Salabas EL, Schüth F: Angew. Chem. Int. Ed.. 2007, 46: 1222. COI number [1:CAS:528:DC%2BD2sXitF2lurs%3D] 10.1002/anie.200602866View ArticleGoogle Scholar
- Varadan VK, Chen LF, Xie JN: Nanomedicine: Design and Applications of Magnetic Nanomaterials. Nanosensors and Nanosystems John Wiley & Sons, Ltd New York; 2008.View ArticleGoogle Scholar
- Sun SH, Zeng H, Robinson DB, Raoux S, Rice PM, Wang SX, Li GX: J. Am. Chem. Soc.. 2004, 126: 273. COI number [1:CAS:528:DC%2BD3sXps1yms7o%3D] 10.1021/ja0380852View ArticleGoogle Scholar
- Sun SH, Zeng H: J. Am. Chem. Soc.. 2002, 124: 8204. COI number [1:CAS:528:DC%2BD38Xks1arurY%3D] 10.1021/ja026501xView ArticleGoogle Scholar
- Xu ZC, Shen CM, Hou YL, Gao HJ, Sun SH: Chem. Mater.. 2009, 21: 1778. COI number [1:CAS:528:DC%2BD1MXksVOjsrg%3D] 10.1021/cm802978zView ArticleGoogle Scholar
- Jana NR, Chen YF, Peng XG: Chem. Mater.. 2004, 16: 3931. COI number [1:CAS:528:DC%2BD2cXnsVaitb8%3D] 10.1021/cm049221kView ArticleGoogle Scholar
- Teng XW, Yang H: J. Am. Chem. Soc.. 2003, 125: 14559. COI number [1:CAS:528:DC%2BD3sXos1Wjs78%3D] 10.1021/ja0376700View ArticleGoogle Scholar
- Park J, An K, Hwang Y, Park JG, Noh HJ, Kim JY, Park JH, Hwang NM, Hyeon T: Nat. Mater.. 2004, 3: 891. COI number [1:CAS:528:DC%2BD2cXhtVehtrjM]; Bibcode number [2004NatMa...3..891P] 10.1038/nmat1251View ArticleGoogle Scholar
- Peng S, Sun SH: Angew. Chem. Int. Ed.. 2007, 46: 4155. COI number [1:CAS:528:DC%2BD2sXmtlOrsb0%3D] 10.1002/anie.200700677View ArticleGoogle Scholar
- Shevchenko EV, Talapin DV, Kotov NA, O′Brien S, Murray CB: Nature. 2006, 439: 55. COI number [1:CAS:528:DC%2BD28Xht1aqsQ%3D%3D]; Bibcode number [2006Natur.439...55S] 10.1038/nature04414View ArticleGoogle Scholar
- Hu FQ, Wei L, Zhou Z, Ran YL, Li Z, Gao MY: Adv. Mater.. 2006, 18: 2553. COI number [1:CAS:528:DC%2BD28XhtFWqtLrO] 10.1002/adma.200600385View ArticleGoogle Scholar
- Hui C, Shen CM, Yang TZ, Bao LH, Tian JF, Ding H, Li C, Gao HJ: J. Phys. Chem. C.. 2008, 112: 11336. COI number [1:CAS:528:DC%2BD1cXot1eru70%3D] 10.1021/jp801632pView ArticleGoogle Scholar
- Pamela CC, Richard AH, Denise RF: Lippincotts Illustrated Reviews: Biochemistry. Lippincott Williams & Wilkins, Philadelphia; 2008.Google Scholar
- Temesghen W, Sherwood PMA: Anal. Bioanal. Chem.. 2002, 373: 601. COI number [1:CAS:528:DC%2BD38XmtVKjs7s%3D] 10.1007/s00216-002-1362-3View ArticleGoogle Scholar
- Li Z, Chen H, Bao HB, Gao MY: Chem. Mater.. 2004, 16: 1391. COI number [1:CAS:528:DC%2BD2cXit1Sqt70%3D] 10.1021/cm035346yView ArticleGoogle Scholar
- Selvakannan PR, Mandal S, Phadtare S, Pasricha R, Sastry M: Langmuir. 2003, 19: 3545. COI number [1:CAS:528:DC%2BD3sXhslSlt7k%3D] 10.1021/la026906vView ArticleGoogle Scholar
- Shelver WL, Kamp LM, Church JL, Rubio FM: J. Agric. Food Chem.. 2007, 55: 3758. COI number [1:CAS:528:DC%2BD2sXksFSns7g%3D] 10.1021/jf0632841View ArticleGoogle Scholar
- Hottenstein CS, Jourdan SW, Hayes MC, Rubio FM, Herzog DP, Lawruk TS: Environ. Sci. Technol.. 1995, 29: 2754. COI number [1:CAS:528:DyaK2MXot1yltb8%3D] 10.1021/es00011a009View ArticleGoogle Scholar